Presentation on theme: "Composites and carbon fibers Topic 2. Reading assignment Askeland and Phule, The Science and Engineering of Materials, 4 th Edition, Ch. 16. Shakelford,"— Presentation transcript:
Composites and carbon fibers Topic 2
Reading assignment Askeland and Phule, The Science and Engineering of Materials, 4 th Edition, Ch. 16. Shakelford, Introduction to Materials Science for Engineers, 6 th Edition, Ch. 14. Chung, Composite Materials, Ch. 2. Chung, Carbon Fiber Composites, Ch. 1, 2 and 3.
Hull made of a sandwich composite Exterior: Kevlar fiber epoxy-matrix composite Interior: Polyvinyl chloride foam
Some examples of composite materials: (a) plywood is a laminar composite of layers of wood veneer, (b) fiberglass is a fiber- reinforced composite containing stiff, strong glass fibers in a softer polymer matrix ( 175), and (c) concrete is a particulate composite containing coarse sand or gravel in a cement matrix (reduced 50%).
Failure mechanisms Failure in fibers (ductile-matrix composites, e.g., polymer-matrix and metal- matrix composites), so a high interfacial strength is desired. Failure in matrix (brittle-matrix composites, e.g., ceramic-matrix and carbon- matrix composites), so a low interfacial strength is desired (to allow cracks to deflect along fiber-matrix interface, thereby allowing fibers to pull out for the purpose of increasing the toughness)
FiberMatrix Fiber pull-out
Two failure modes in ceramic-ceramic composites: (a) Extensive pull-out of SiC fibers in a glass matrix provides good composite toughness (x20). (b) Bridging of some fibers across a crack enhances the toughness of a ceramic-matrix composite (unknown magnification).
Fracture toughness Increased by reinforcement
Specific strength = strength/density
Reasons for fiber-matrix interface engineering To control fiber-matrix bond strength (shear bond strength) To improve wetting of matrix precursor on fiber To improve fiber dispersion
Methods for fiber-matrix interface engineering Fiber surface treatment Dispersant as an additive to the matrix
Methods of fiber surface treatment Chemical treatment fiber Coating of fiber
Table 2.2 Effects of various surface treatments on properties of high-modulus carbon fibers and their epoxy- matrix composites. Fiber propertiesComposite properties Fiber treatmentWt. loss (%) Tensile strength loss (%) Flexural strength loss (%) ILSS gain (%) 400ºC in air (30 min) ºC in air (30 min) ºC in air (30 min)4.550Too weak to test- 60% HNO 3 (15 min) % NaOCl (30 min) % NaOCl (15 min) % HClO 4 (15 min) % KMnO 4 /10% NaOH (15 min) % KMnO 4 /10% H 2 SO 4 (15 min)6.0(+) % H 2 O 2 /20% H 2 SO 4 (15 min) % HNO 3 /30% H 2 SO 4 (15 min)0.104(+)0 10% NaClO 3 /15% NaOH (15 min) % NaClO 3 /25% H 2 SO 4 (15 min)0.225(+)91 15% NaClO 3 /40% H 2 SO 4 (15 min) % Na 2 Cr 2 O 7 /25% H 2 SO 4 (15 min)0.3815(+)18 15% Na 2 Cr 2 O 7 /40% H 2 SO 4 (15 min) All liquid treatments at reflux temperature.
Types of polymer-matrix composites Thermoplastic-matrix composites Thermoset-matrix composites
Lower manufacturing cost of thermoplastic-matrix composites no cure unlimited shelf-life reprocessing possible (for repair and recycling) less health risks due to chemicals during processing low moisture content thermal shaping possible weldability (fusion bonding possible)
Better performance of thermoplastic-matrix composites high toughness (damage tolerance) good hot/wet properties high environmental tolerance
Disadvantages of thermoplastic-matrix composites limitations in processing methods high processing temperatures high viscosities prepreg (collection of continuous fibers aligned to form a sheet which has been impregnated with the polymer or polymer precursor) being stiff and dry when solvent is not used (i.e., not drapeable or tacky) fiber surface treatments less developed
Attractive properties of carbon fiber polymer-matrix composites low density (40% lower than aluminum) high strength (as strong as high-strength steels) high stiffness (stiffer than titanium, yet much lower in density) good fatigue resistance (a virtually unlimited life under fatigue loading) good creep resistance
Attractive properties of carbon fiber polymer-matrix composites low friction coefficient and good wear resistance (a 40 wt.% short carbon fiber nylon-matrix composite has a friction coefficient nearly as low as Teflon and unlubricated wear properties approaching those of lubricated steel) toughness and damage tolerance (can be designed by using laminate orientation to be tougher and much more damage tolerant than metals) chemical resistance (chemical resistance controlled by the polymer matrix) corrosion resistance (impervious to corrosion)
Attractive properties of carbon fiber polymer-matrix composites dimensional stability (can be designed for zero coefficient of thermal expansion) vibration damping ability (excellent structural damping when compared with metals) low electrical resistivity high electromagnetic interference (EMI) shielding effectiveness high thermal conductivity
Limitation of polymer- matrix composites Inability to resist high temperatures
Carbon-matrix composites Ability to resist high temperatures
Carbon-carbon (C/C) composites Carbon fiber Carbon matrix Carbon matrix made from pitch or polymer
Conversion of carbon matrix precursor to carbon Pyrolysis (also called carbonization) Heating at around 1000°C in the absence of oxygen to cause decomposition, like charring
Bonding in graphite In-plane: covalent and metallic bonding Out-of-plane: van der Waals bonding
Properties of graphite Anisotropic Easy shear between carbon layers limiting the strength High electrical and thermal conductivity and high modulus in the plane of the carbon layers
Fiber microstructure Fiber texture, i.e., preferred crystallographic orientation with the carbon layers along the fiber axis.
Carbon Non-crystalline, turbostratic Metastable form – graphitizes upon heating above 2000°C.
Conversion of carbon to graphite Graphitization (i.e., crystallization) Heating at 2000°C or above in the absence of oxygen to cause the turbostratic carbon to be converted to graphite (crystalline)
Properties of carbon compared to graphite Less conductive Lower in modulus Higher in strength Lower in oxidation resistance Cannot be intercalated
Fiber vs. nanofiber Fiber (diameter 1 micron or above, typically around 10 microns) Nanofiber (also called filament, diameter below 1 micron, typically 0.1 micron or less)
Types of carbon nanofiber Nanofiber with fish-bone morphology Multi-walled nanotube (concentric cylinders in shell) Single-walled nanotube (chirality)
Carbon nanotube Hybrid of graphite and fullerene
Crystal forms of carbon Graphite Diamond Fullerene
Nanofiber group morphology Intertwined Parallel
Fabrication of carbon nanofibers Catalytic growth from carbonaceous gas Arc discharge Laser evaporation
Catalytic method Carbonaceous gases: acetylene, ethylene, methane, natural gas, benzene, etc. Catalyst: iron, nickel, etc. (particles typically 10 nm, from salts or organometallics) Reducing gases: CO, hydrogen
Methods of making carbon- carbon composites Carbonization, followed by impregnation of pitch or resin, and repeating the carbonization- impregnation process again and again until sufficient density has been attained. Chemical vapor infiltration (CVI) using a carbonaceous gas, i.e., CVD under a temperature/pressure gradient so as to prevent crust formation, thereby allowing complete infiltration; CVI can be an extra step that follows carbonization-impregnation for the purpose of filling the pores.
Table 2.3 Pitch properties. Carbon yield (%) PitchMolecular weight 0.1 MPa10 MPa A B C
Grades of pitch Isotropic pitch Mesophase pitch (liquid crystal form called the mesophase)
Main problem with carbon-carbon composites Oxidation at high temperatures in the presence of oxygen
Methods for oxidation protection of carbon-carbon composites up to 1700 C 1.SiC conversion coating 2.Oxidation inhibitors 3.Glassy sealant 4.Dense SiC or Si 3 N 4 overlayer on glassy sealant or SiC conversion coating
SiC conversion coating method SiC coating (known as SiC conversion coating, due to graded composition from pure SiC at the surface to pure carbon inside)
Methods of applying SiC conversion coating - Pack cementation, - Reaction sintering, - Silicone resin impregnation/pyrolysis, or - Chemical vapor deposition (CVD) to the outer surface of the composite.
Pack cementation Packing the composite in a mixture of SiC and Si powders and heat up to 1600°C Chemical conversion of the outermost surface of the composite to SiC SiC coating thickness typically mm.
Si(l) + C SiC Si(g) + C SiC SiO(g) + 2C SiC + CO(g) Pack cementation Problem with entrapped silicon vaporising.
Reaction sintering Dipping C/C composite into a suspension of Si powder (10 μm) in an alcohol solution and then sintering at 1600°C for 4 hours in argon.
Silicone resin impregnation/pyrolysis Vacuum impregnation and cold isostatic pressing (30,000 psi or 200 MPa) a silicone resin into the matrix of a C/C composite and subsequent pyrolysis at 1600°C for 2 hours in argon. Note: Silicone is a polymer with silicon atoms as a part of the backbone.
Prior deposition of carbon film (10 μm) by CVD Prior to pack cementation, reaction sintering or resin impregnation To improve homogeneity of C/C surface To ease the reaction with Si
Dense SiC or Si 3 N 4 overlayers SiC overlayer is more dense than the SiC conversion coating. As oxygen barrier To control venting of reaction products to the outside Made by chemical vapor deposition (CVD)
CH 3 SiCl 3 (g) SiC + 3HCl(g) Heat/H 2 Chemical vapor deposition (CVD) by thermal decomposition of a volatile silicon compound Temperature: 1125°C
SiSiC overlayer CVD overlayer contains a small percentage of unreacted silicon dispersed in the SiC, The excess Si upon oxidation becomes SiO 2, which has a very low oxygen diffusion coefficient.
Advantages of SiC or Si 3 N 4 Thermal expansion compatibility with C/C Low oxidation rate Thin amorphous SiO 2 scale that grows has low oxygen diffusion coefficient.
SiC or ineffective above 1800°C Reactions at the interface between SiO 2 and SiC or Si 3 N 4 Reduction of SiO 2 by carbon to form CO gas.
Oxygen inhibitors Oxygen getters Glass formers To provide additional oxidation protection from within by migrating to the outer surface and sealing cracks and voids during oxidation.
Examples of inhibitors Elemental Si, Ti and B SiC, Ti 5 Si 3 and TiB 2 Alloys such as Si 2 TiB 14 Organoborosilazane polymer solution Oxidation of the elemental Si, Ti or B within the carbon matrix forms a viscous glass, which serves as a sealant that flows into the microcracks of the SiC coating.
Boron as an oxidation inhibitor Boron is oxidized to form B 2 O 3. B 2 O 3 blocks active sites, such as the edge carbon atoms. B 2 O 3 forms a mobile diffusion barrier for oxygen.
Oxidation rate Rate of weight loss
Inhibition factor Ratio of oxidation rate of untreated carbon to that of the treated carbon
Incorporating particulate fillers in the resin or pitch (i) prior to prepregging. during lay-up and (ii) during densification cycles. Method of introducing oxidation inhibitors to the carbon matrix
Glassy sealants Glazes comprising mainly silicates (SiO x ) and borates (B 2 O 3 ). Glaze can be filled with SiC particles Particularly important if the SiC conversion coating is porous Glaze fills microcracks in the dense overlayer
Application of a glassy sealant on top of the SiC conversion coating mainly by slurry brush-on, so that the sealants melt, fill voids and stop oxygen diffusion, and, in some cases, act as oxygen getters.
Effectiveness of borate sealants Borates wet C and SiC quite well Borates cannot be used above 1200°C due to volatilization Borates have poor moisture resistance due to hydrolysis, which results in swelling and crumbling Borate has a tendency to galvanically corrode SiC coatings at high temperatures
Modified borate sealants The problems of borate can be alleviated by using multicomponent systems such as 10TiO 2.20SiO 2.70B 2 O 3. TiO 2 has a high solubility in B 2 O 3 and is used to prevent the volatilization of B 2 O 3 and increase the viscosity. SiO 2 acts to increase the moisture resistance, reduce B 2 O 3 volatility, increase viscosity and prevent corrosion of SiC by B 2 O 3.
Dense SiC or Si 3 N 4 overlayer Applied by CVD. On top of glassy sealant or on top of SiC conversion coating To control and inhibit transfer of oxygen to the substrate To control the venting of reaction products to the outside
Method of oxidation protection of C/C above 1700°C Four-layer coating scheme: (1) Refractory oxide (e.g., ZrO 2, HfO 2, Y 2 O 3, ThO 2 ) as the outer layer for erosion protection. (2) SiO 2 glass inner layer as and oxygen barrier and sealant. (3) Another refractory oxide layer for isolation of the SiO 2 from the carbide layer underneath. (4) Refractory carbide layer (e.g., TaC, TiC, HfC, ZrC) to interface with the C/C substrate and to provide a carbon diffusion barrier
Fundamental approaches for oxidation protection of carbons Prevention of catalysis Retardation of gas access to the carbon Inhibition of carbon-gas reactions Improvement in the carbon crystalline structure
Carbon matrix precursors Pitch (preferred for oxidation protection) Chemical vapor infiltration (CVI) carbon (preferred for oxidation protection) Resins (not preferred for oxidation protection)
Effects of carbon fiber on oxidation protection Alignment of the matrix molecules near the fibers Microstructure of fiber affecting that of matrix Microstructure of matrix affecting amount of accessible porosity in the matrix
Disadvantage of coatings on C/C Degrade room temperature mechanical properties of C/C
Metal-matrix composites Better temperature resistance than polymer-matrix composites Lower temperature resistance than ceramic-matrix composites High fabrication cost compared to polymer-matrix composites Low fabrication cost compared to ceramic-matrix composites
Methods of fabricating metal-matrix composites Liquid metal infiltration Hot pressing above the solidus of the matrix metal Powder metallurgy (diffusion bonding) Plasma spraying Slurry casting
Advantages of liquid metal infiltration Near-net shape Fast
Difficulty in liquid metal infiltation Liquid metal does not wet ceramic or carbon particles/fibers well.
Reaction between metal and reinforcement Helps wetting Degrades reinforcement Reaction product (e.g., a carbide) lining the metal- reinforcement interface may be brittle
Methods of wetting enhancement Coat reinforcement with a metal (e.g., Ni, Cu, Ag) by plating Coat reinforcement with a ceramic (e.g., TiC, SiC, B 4 C, TiB 2, TiN, K 2 ZrF 6, ZrO 2 ) by CVD, solution coating, etc.
Coating of TiB 2 on carbon fiber by CVD TiCl 4 and BCl 3 gases, which are reduced by zinc vapor Coating particularly good for liquid aluminum
Solution coating method Dip in organometallic solution (e.g., alkoxides, which are M(OR) x, where M is the metal, and R is a hydrocarbon group, such as methyl, ethyl, etc.) Hydrolysis or pyrolysis to organometallic compounds
Si(OC 2 H 5 ) 4 + 2H 2 O SiO 2 + 4C 2 H 5 OH Hydrolysis of organometallic compound
Si(OC 2 H 5 ) 4 SiO 2 + 2C 2 H 5 OH + 2C 2 H 4 Pyrolysis of organometallic compound
Powder metallurgy Near-net shape Size limited by the pressure requirement
Two methods of powder metallurgy Mixture of matrix powder and reinforcement particles/fibers Matrix coated reinforcement particles/fibers